Hindawi Publishing Corporation International Journal of Biomaterials Volume 2015, Article ID 921425, 6 pages http://dx.doi.org/10.1155/2015/921425
Research Article Effect of Bleaching and Thermocycling on Resin-Enamel Bond Strength Horieh Moosavi,1 Hamideh Sadat Mohammadipour,1 Marjaneh Ghavamnasiri,2 and Sanaz Alizadeh1 1
Dental Materials Research Center and Department of Operative Dentistry, Faculty of Dentistry, Mashhad University of Medical Sciences, Mashhad 91735, Iran 2 Dental Research Center, Department of Operative Dentistry, Mashhad Dental School, Mashhad University of Medical Sciences, Mashhad 91735, Iran Correspondence should be addressed to Sanaz Alizadeh; [email protected]
Received 4 October 2015; Revised 28 November 2015; Accepted 1 December 2015 Academic Editor: Vijaya K. Rangari Copyright © 2015 Horieh Moosavi et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. The aim of this study was to evaluate the effect of bleaching and thermocycling on microshear bond strength of bonded resin composites to enamel. Enamel slices were prepared from ninety-six intact human premolars and resin composite cylinders were bonded by using Adper Single Bond 2 + Filtek Z350 or Filtek silorane adhesive and resin composite. Each essential group was randomly subdivided to two subgroups: control and bleaching. In bleaching group, 35% hydrogen peroxide was applied on samples. Thermocycling procedure was conducted between 5∘ C and 55∘ C, for 3.000 cycles on the half of each subgroup specimen. Then microshear bond strength was tested. Methacrylate-based resin composite had higher bond strength than silorane-based one. The meyhacrylate-based group without bleaching along with thermocycling showed the most bond strength, while bleaching with 35% carbamide peroxide on silorane-based group without thermocycling showed the least microshear bond strength. Bleaching caused a significant degradation on shear bond strength of silorane-based resin composites that bonded using self-etch adhesive resin systems.
1. Introduction Bleaching popularity and introducing the new bleaching products every year lead to many studies about the effects of these products on teeth and dental restorative materials. Effects of free radicals releasing during bleaching process on physicomechanical properties of restorations such as their colour, surface roughness, strength, hardness, and ion leakage are subjects of most scientists’ discussions . Conventional composites have marked polymerization shrinkage because of Bis-GMA monomers, but silorane-based composites showed less shrinkage, thus microleakage and its side effects are less. However a previous study showed that restorations of both materials were clinically acceptable after 5 years . It was shown that bleaching of fluorosed teeth reduces bracket bond strength to enamel, but the bond strength with these still exceeds the minimum . It has
been stated that bond strength of restorations to enamel and dentin was affected by carbamide peroxide and this defect was related by carbamide peroxide concentration . Just some articles showed bleaching agents could penetrate pulp chamber through composite restorations [5, 6]. In addition, it was suggested that bleaching could adversely affect the interfacial fracture toughness of dentin-resin composite adhesive interfaces . The other studies showed increasing marginal leakage in postoperative bleaching of class V resin composite restorations [8, 9]. However, it was found that immediate postoperative bleaching with 20% carbamide peroxide gel, 6% hydrogen peroxide, and 19% percarbonate gel for 14 days had no influence on microleakage of Filtek composite bonded with Scotchbond 1 at the occlusal margins of the Class 1 restorations . Composite materials may be failed by mechanical and thermocycling (TC) condition, interfacial debonding, microcracking, and filler particle fracture,
International Journal of Biomaterials
M (control) n = 24 M (Filtek Z350) n = 48 samples
MB (bleaching) n = 24 96 premolars S (control) n = 24 S (Filtek silorane) n = 48 samples
SB (bleaching) n = 24
MT (with thermocycling) n = 12 M (without thermocycling) n = 12
MBT (with thermocycling) n = 12 MB (without thermocycling) n = 12 ST (with thermocycling) n = 12 S (without thermocycling) n = 12
SBT (with thermocycling) n = 12 SB (without thermocycling) n = 12
Figure 1: The schematic of experimental groups.
which could reduce the survival probability of composite restorations in vivo . Numerous in vitro studies of the mechanical performance of dental composite materials after TC showed that artificial aging protocols accelerate degradation of materials, which significantly degrades mechanical properties [11–16]. In contrast, Smisson et al. found no significant differences in the mechanical properties (flexural strength and bond strength) of a hybrid resin composite tested under five different TC protocols . A recent review concluded that there was no standardized TC protocol to reproduce aging conditions in the oral cavity . As far as the authors are aware, effects of contemporary bleaching and thermocycling on bonded composites were a few in previous studies, to date. Therefore, the aim of this study is to evaluate the effect of bleaching and thermocycling on microshear bond strength of bonded dimethacrylate and silorane-based resin composites to enamel. The null hypotheses were that the bonded composites are not significantly influenced by (1) type of resin composite or (2) bleaching procedure or (3) thermocycling regimen.
2. Materials and Methods 2.1. Specimen Preparation. Ninety-six intact premolars had been extracted for orthodontic reasons that were gathered following informed consent approved by the Commission for Medical Ethics of the University of Medical Sciences (N#901114). The remaining soft tissue, calculus, and plaque were removed with rubber cap and slurry of pumice after hand scaling instrument and then stored in 0.1% thymol solution until operation time. One millimeter thickness of enamel slices was prepared parallel to proximal surfaces and polished by 200, 400, and 600 grit silicon carbide papers (3M, St. Paul, USA) under water cooling, respectively. Samples were divided into two groups based on resin composite types (𝑛 = 48); nanofill resin composite with dimethacrylate base (3M ESPE, Filtek Z350 Universal Restorative Dental
Products, St. Paul, USA) (group M) and silorane-based resin composite (3M ESPE, Filtek silorane, Dental Products, St. Paul, USA) (group S). For the groups restored with the dimethacrylate material (group M), enamel surface was etched by 37% phosphoric acid gel for 30 seconds (3M ESPE, Scotchbond Etchant, Dental Products, St. Paul, USA), rinsed with water/air syringe for 30 seconds, and dried gently with air syringe only for 5 seconds. Then, two consecutive coats of Single Bond adhesive (3M ESPE, Adper, Dental Products, St. Paul, USA) were applied on etched surface. Each layer was gently air dried for 5 seconds to make a delicate and shiny surface and light cured for 20 seconds by light cure device with 500 mW/cm2 intensity (Blue phase C8, Vivadent Ivoclare, Austria). The groups were restored with the siloranebased composite resin (Filtek silorane; group S), each Silorane System Adhesive Self-Etch Primer and Bond (3M ESPE, Dental Products, St. Paul, USA) was applied according the manufacture’s instruction (Table 1). In all samples, before adhesive curing, silicon tubes with an internal diameter of 0.7 mm and a height of ∼2 mm were placed on the adhesive surface and then the adhesives were light-cured. Composites were incrementally condensed in tubes, by a plastic instrument in two 1 mm layers and each layer was polymerized for 40 seconds. After 24 hours, silicon tubes were removed by using a scalpel (Fine science tools GmbH, Germany) with a number 11 blade (Fine science tools GmbH, Germany). Half samples of each resin composite were bleached by 35% hydrogen peroxide (Opalescence Endo, Ultradent Products, USA) which was used for 3 ∗ 20 minutes, according to manufacturer’s instruction. So both resin composite types were divided into two subgroups (𝑛 = 24): control (C) and bleaching (B). The half of each resin composite subgroups (𝑛 = 12) was subjected to thermocycling (T) process (custom procedure made by NIOM-Scandinavian Institute for Dental Materials, Haslum, Norway) for 3.000 cycles between 5∘ C and 55∘ C in deionized water with a dwell time of 30 seconds and transfer time of 10 seconds (Figure 1). Samples were stored in
International Journal of Biomaterials
Table 1: Materials, chemical compositions, and manufacturer used in the study. Material
Filtek Z350 resin composite
Filtek silorane resin composite (P90)
Adper Single Bond 2
Silorane System Adhesive Self-Etch Primer
Silorane System Adhesive Bond Opalescence Endo
Components BIS-GMA, BIS-EMA (6), UDMA, and TEGDMA, a nonagglomerated/nonaggregated, 20 nm nanosilica filler, loosely bound agglomerated zirconia/silica nan cluster, consisting of agglomerates of primary zirconia/silica particles with size of 5–20 nm fillers (82% wt) Silane-treated quartz, 3,4-epoxycyclohexylcyclopolymethylsiloxane, yttrium trifluoride, bis-3,4-epoxycyclohexylethyl-phenylmethylsilane, mixture of epoxy functional di- and oligo-siloxane by-products, mixture of alpha substituted by-products, mixture of other byproducts, and mixture of epoxy-mono-silanole byproducts (79% wt) 32% phosphoric acid, fumed silica, and water BisGMA, HEMA, dimethacrylates, ethanol, water, a novel photoinitiator system and a methacrylate functional copolymer of polyacrylic and polyitaconic acids, and silica particles 2-Hydroxyethyl methacrylate (HEMA), bisphenol A diglycidyl ether dimethacrylate (BisGMA), water, ethanol, phosphoric acid-methacryloxy-hexyl esters, silane-treated silica, 1,6-hexanediol dimethacrylate, copolymer of acrylic and itaconic acid, (dimethylamino)ethyl methacrylate, DL-camphorquinone, phosphine oxide Substituted dimethacrylate, silane-treated silica, triethylene glycol dimethacrylate (tegdma), phosphoric acid methacryloxy-hexyl esters, 1,6-hexanediol dimethacrylate, and DL-camphorquinone
Manufacturer 3M ESPE, Filtek Z350 Universal Restorative Dental Products, St. Paul, USA
3M ESPE, Filtek silorane, Dental Products, St. Paul, USA
3M ESPE, Scotchbond Etchant, Dental Products, St. Paul, USA 3M ESPE, Adper Single Bond 2 adhesive, Dental Products, St. Paul, USA
3M ESPE, Dental Products, St. Paul, USA
3M ESPE, Dental Products, St. Paul, USA Ultradent Products Inc., USA
35% hydrogen peroxide
HEMA: 2-hydroxyethyl methacrylate; Bis-GMA: bisphenol A diglycidyl methacrylate; TEGDMA: triethylene glycol dimethacrylate; BIS-EMA: ethoxylated bisphenol A glycol dimethacrylate; UDMA: urethane dimethacrylate. The “number (6) and (90)” are as the chemical formulation or the part of name of “BIS-EMA” and “Filtek Silorane resin composite” respectively.
artificial saliva in 37∘ C prior to microshear bond strength test. The shear-bond strength was measured with Universal testing machine (SANTAM STM-20, Santam, Iran). A knife edge shearing rod with a crosshead speed of 0.5 mm/min and 6 kg load cell was used. It was recorded the load at failure for each specimen. The microshear bond strength of the specimens were calculated and expressed in MPa. The failure mode of each beam was examined under a stereomicroscope (DinoLite Pro, AnMo Electronics Corp, Taiwan) at a magnification of up to 50x. Failures were categorized as cohesive (occurring within dentin or composite), adhesive (occurring between the two materials), or mixed (a combination of cohesive and adhesive). 2.2. Statistical Analysis. All statistics were performed with SPSS version 11.0.0 (SPSS Inc., Chicago, IL, USA). The Kolmogorov-Smirnov test confirmed the normal distribution
of the data, and a parametric approach was used to verify the null hypotheses. Interaction among study variables (type of composite with regarding to adhesive, bleaching, and thermal cycling) was tested by ANOVA with Tukey’s post hoc multiple-comparison tests. The significance level was set at 𝛼 = 0.05.
3. Results The mean and standard deviations of each group are displayed in Table 2. Maximum and minimum of bond strength were observed in groups MT and SB, respectively. According to analysis of variance there was an interaction among three variables: composite type, bleaching, and thermocycling. Thermocycling caused an increasing in shear bond strength of control groups and bleaching by 35% hydrogen peroxide
International Journal of Biomaterials
Table 2: Mean values and respective standard deviations of microshear bond strength (MPa) in experimental groups. Experimental groups abbreviation Filtek Z350 resin composite (group M) MT M MBT MB Filtek silorane resin composite (group S) ST S SBT SB 𝑃 value
44.64a 18.18b 39.93a 21.09b
11.62 5.68 11.03 4.79
26.33b 16.56bc 24.20b 9.73d
8.61 3.55 7.60 2.38